LMucko/crystallography-open-database huggingface dataset:
Zur Kristallstruktur von Cu3 Nb Ta O8
Harneit, O; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 613 (1992) 60–62; doi:10.1002/zaac.19926130110

data_2002583
_publ_section_title              'Zur Kristallstruktur von Cu3 Nb Ta O8'
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              60
_journal_page_last               62
_journal_paper_doi               10.1002/zaac.19926130110
_journal_volume                  613
_journal_year                    1992
_chemical_formula_structural     'Cu3 (Nb Ta O8)'
_chemical_formula_sum            'Cu3 Nb O8 Ta'
_chemical_name_systematic        'Tricopper niobotantalate'
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                72.85(7)
_cell_angle_beta                 83.39(5)
_cell_angle_gamma                65.77(3)
_cell_formula_units_Z            1
_cell_length_a                   5.179(5)
_cell_length_b                   5.474(6)
_cell_length_c                   6.003(5)
_cell_volume                     148.3
_refine_ls_R_factor_all          0.043
_cod_database_code               2002583
Zur Kenntnis von Cu6 La4 Mo9 O36
Krueger, T F; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 614 (1992) 35–37; doi:10.1002/zaac.19926140808

data_2002584
_publ_section_title              'Zur Kenntnis von Cu6 La4 Mo9 O36'
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              35
_journal_page_last               37
_journal_paper_doi               10.1002/zaac.19926140808
_journal_volume                  614
_journal_year                    1992
_chemical_formula_structural     'Cu6 La4 (Mo O4)9'
_chemical_formula_sum            'Cu6 La4 Mo9 O36'
_chemical_name_systematic
;
Hexacopper(I) tetralanthanum nonakis(molybdate)
;
_space_group_IT_number           161
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3 -2"c'
_symmetry_space_group_name_H-M   'R 3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   20.892(5)
_cell_length_b                   20.892(5)
_cell_length_c                   12.754(5)
_cell_volume                     4821.0
_refine_ls_R_factor_all          0.085
_cod_original_sg_symbol_H-M      'R 3 c H'
_cod_database_code               2002584
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2 O8
Postel, M von; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 615 (1992) 97–100; doi:10.1002/zaac.19926150919

data_2002585
_publ_section_title
;
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2
O8
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              97
_journal_page_last               100
_journal_paper_doi               10.1002/zaac.19926150919
_journal_volume                  615
_journal_year                    1992
_chemical_formula_structural     'Ba (Mg Zn) (V O4)2'
_chemical_formula_sum            'Ba Mg O8 V2 Zn'
_chemical_name_systematic        'Barium magnesium zinc bis(vanadate)'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I 4bw 2aw -1bw'
_symmetry_space_group_name_H-M   'I 41/a c d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.4524(57)
_cell_length_b                   12.4524(57)
_cell_length_c                   8.4408(36)
_cell_volume                     1308.8
_refine_ls_R_factor_all          0.047
_cod_original_sg_symbol_H-M      'I 41/a c d S'
_cod_database_code               2002585
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2 O8
Postel, M von; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 615 (1992) 97–100; doi:10.1002/zaac.19926150919

data_2002586
_publ_section_title
;
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2
O8
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              97
_journal_page_last               100
_journal_paper_doi               10.1002/zaac.19926150919
_journal_volume                  615
_journal_year                    1992
_chemical_formula_structural     'Ba Mn2 (V O4)2'
_chemical_formula_sum            'Ba Mn2 O8 V2'
_chemical_name_systematic        'Barium dimanganese bis(vanadate)'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I 4bw 2aw -1bw'
_symmetry_space_group_name_H-M   'I 41/a c d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.5563(14)
_cell_length_b                   12.5563(14)
_cell_length_c                   8.5942(9)
_cell_volume                     1355.0
_refine_ls_R_factor_all          0.047
_cod_original_sg_symbol_H-M      'I 41/a c d S'
_cod_database_code               2002586
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2 O8
Postel, M von; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 615 (1992) 97–100; doi:10.1002/zaac.19926150919

data_2002587
_publ_section_title
;
Zur Kenntnis von Ba (Mg Zn) V2 O8, Ba Mn2 V2 O8 und Ba1/2 Sr1/2 Ni2 V2
O8
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              97
_journal_page_last               100
_journal_paper_doi               10.1002/zaac.19926150919
_journal_volume                  615
_journal_year                    1992
_chemical_formula_structural     '(Ba0.5 Sr0.5) Ni2 (V O4)2'
_chemical_formula_sum            'Ba0.5 Ni2 O8 Sr0.5 V2'
_chemical_name_systematic
;
Hemibarium hemistrontium dinickel bis(vanadate)
;
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I 4bw 2aw -1bw'
_symmetry_space_group_name_H-M   'I 41/a c d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.2248(20)
_cell_length_b                   12.2248(20)
_cell_length_c                   8.3245(15)
_cell_volume                     1244.1
_refine_ls_R_factor_all          0.057
_cod_original_sg_symbol_H-M      'I 41/a c d S'
_cod_original_formula_sum        'Ba.5 Ni2 O8 Sr.5 V2'
_cod_database_code               2002587
Eine weitere Oxovanadat-Phase mit Granatstruktur: Ca5 Mg3 Zn V6 O24
Mueller-Buschbaum, Hk; Postel, M von; Zeitschrift fuer Anorganische und Allgemeine Chemie 615 (1992) 101–103; doi:10.1002/zaac.19926150920

data_2002588
_publ_section_title
;
Eine weitere Oxovanadat-Phase mit Granatstruktur: Ca5 Mg3 Zn V6 O24
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              101
_journal_page_last               103
_journal_paper_doi               10.1002/zaac.19926150920
_journal_volume                  615
_journal_year                    1992
_chemical_formula_structural     'Ca5 Mg3 Zn (V O4)6'
_chemical_formula_sum            'Ca5 Mg3 O24 V6 Zn'
_chemical_name_systematic
;
Pentacalcium trimagnesium zinc hexakis(vanadate)
;
_space_group_IT_number           220
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.4292(11)
_cell_length_b                   12.4292(11)
_cell_length_c                   12.4292(11)
_cell_volume                     1920.1
_refine_ls_R_factor_all          0.049
_cod_database_code               2002588
Ds erste Erdalkalimetall-Mercurato(II)-Palladat(II,IV): Ba2 Hg3 (Pd2+)5 (Pd4+)2 O14
Hansen, Th; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 616 (1992) 67–70; doi:10.1002/zaac.19926161011

data_2002589
_publ_section_title
;
Ds erste Erdalkalimetall-Mercurato(II)-Palladat(II,IV): Ba2 Hg3 (Pd2+)5
(Pd4+)2 O14
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              67
_journal_page_last               70
_journal_paper_doi               10.1002/zaac.19926161011
_journal_volume                  616
_journal_year                    1992
_chemical_formula_structural     'Ba2 (Hg3 Pd5 Pd2 O14)'
_chemical_formula_sum            'Ba2 Hg3 O14 Pd7'
_chemical_name_systematic
;
Dibarium trimercuropentapalladodipalladate(IV)
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.56(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.583(2)
_cell_length_b                   6.207(4)
_cell_length_c                   10.919(4)
_cell_volume                     717.2
_refine_ls_R_factor_all          0.043
_cod_database_code               2002589
Das erste Alkali-Erdalkali-Oxocuprat (II,III): Na Ba2 (Cu2+)2 (Cu3+) O6
Tams, G; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 19–22; doi:10.1002/zaac.19926170103

data_2002590
_publ_section_title
;
Das erste Alkali-Erdalkali-Oxocuprat (II,III): Na Ba2 (Cu2+)2 (Cu3+) O6
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              19
_journal_page_last               22
_journal_paper_doi               10.1002/zaac.19926170103
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Na Ba2 Cu2 Cu O6'
_chemical_formula_sum            'Ba2 Cu3 Na O6'
_chemical_name_systematic        'Sodium dibarium dicopper copper(III) oxide'
_space_group_IT_number           69
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      69
_symmetry_space_group_name_Hall  '-F 2 2'
_symmetry_space_group_name_H-M   'F m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.4229(22)
_cell_length_b                   11.4418(32)
_cell_length_c                   14.4063(47)
_cell_volume                     1388.4
_refine_ls_R_factor_all          0.044
_cod_database_code               2002590
Zur Kenntnis eines Oxoargentato(I)-aurats(III):Ba4 Ag Au O6
Weinreich, J; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 27–30; doi:10.1002/zaac.19926170105

data_2002591
_publ_section_title
;
Zur Kenntnis eines Oxoargentato(I)-aurats(III):Ba4 Ag Au O6
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              27
_journal_page_last               30
_journal_paper_doi               10.1002/zaac.19926170105
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Ba4 (Ag O2) (Au O4)'
_chemical_formula_sum            'Ag Au Ba4 O6'
_chemical_name_systematic        'Tetrabarium dioxoargentate tetraoxoaurate'
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.2751(33)
_cell_length_b                   5.7820(15)
_cell_length_c                   11.3961(22)
_cell_volume                     874.7
_refine_ls_R_factor_all          0.069
_cod_database_code               2002591
Ein Beitrag zur Kristallstruktur von Cu Sm Mo2 O8 und Cu Gd Mo2 O8
Krueger, T F; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 79–83; doi:10.1002/zaac.19926170112

data_2002592
_publ_section_title
;
Ein Beitrag zur Kristallstruktur von Cu Sm Mo2 O8 und Cu Gd Mo2 O8
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              79
_journal_page_last               83
_journal_paper_doi               10.1002/zaac.19926170112
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Cu Sm (Mo O4)2'
_chemical_formula_sum            'Cu Mo2 O8 Sm'
_chemical_name_systematic        'Copper(I) samarium bis(molybdate)'
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.302(3)
_cell_length_b                   9.796(5)
_cell_length_c                   14.697(6)
_cell_volume                     1483.2
_refine_ls_R_factor_all          0.063
_cod_database_code               2002592
Ein Beitrag zur Kristallstruktur von Cu Sm Mo2 O8 und Cu Gd Mo2 O8
Krueger, T F; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 79–83; doi:10.1002/zaac.19926170112

data_2002593
_publ_section_title
;
Ein Beitrag zur Kristallstruktur von Cu Sm Mo2 O8 und Cu Gd Mo2 O8
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              79
_journal_page_last               83
_journal_paper_doi               10.1002/zaac.19926170112
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Cu Gd (Mo O4)2'
_chemical_formula_sum            'Cu Gd Mo2 O8'
_chemical_name_systematic        'Copper(I) gadolinium bis(molybdate)'
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.200(7)
_cell_length_b                   9.779(7)
_cell_length_c                   14.646(45)
_cell_volume                     1460.9
_refine_ls_R_factor_all          0.069
_cod_database_code               2002593
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2 Fe4 O15 und Ba5 Ca Nd2 Co4 O15
Mueller-Buschbaum, Hk; Martin, F - D; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 84–88; doi:10.1002/zaac.19926170113

data_2002594
_publ_section_title
;
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2
Fe4 O15 und Ba5 Ca Nd2 Co4 O15
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              84
_journal_page_last               88
_journal_paper_doi               10.1002/zaac.19926170113
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Ba4.5 Ca1.5 La2 Fe4 O15'
_chemical_formula_sum            'Ba4.5 Ca1.5 Fe4 La2 O15'
_chemical_name_systematic
;
Barium calcium lanthanum iron(III) oxide (4.5/1.5/2/4/15)
;
_space_group_IT_number           186
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.6771(42)
_cell_length_b                   11.6771(42)
_cell_length_c                   6.9593(50)
_cell_volume                     821.8
_refine_ls_R_factor_all          0.06
_cod_database_code               2002594
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2 Fe4 O15 und Ba5 Ca Nd2 Co4 O15
Mueller-Buschbaum, Hk; Martin, F - D; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 84–88; doi:10.1002/zaac.19926170113

data_2002595
_publ_section_title
;
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2
Fe4 O15 und Ba5 Ca Nd2 Co4 O15
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              84
_journal_page_last               88
_journal_paper_doi               10.1002/zaac.19926170113
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Ba5 Ca Eu2 Fe4 O15'
_chemical_formula_sum            'Ba5 Ca Eu2 Fe4 O15'
_chemical_name_systematic
;
Pentabarium calcium dieuropium tetrairon(III) oxide
;
_space_group_IT_number           186
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.5701(23)
_cell_length_b                   11.5701(23)
_cell_length_c                   6.8916(55)
_cell_volume                     799.0
_refine_ls_R_factor_all          0.053
_cod_database_code               2002595
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2 Fe4 O15 und Ba5 Ca Nd2 Co4 O15
Mueller-Buschbaum, Hk; Martin, F - D; Zeitschrift fuer Anorganische und Allgemeine Chemie 617 (1992) 84–88; doi:10.1002/zaac.19926170113

data_2002596
_publ_section_title
;
Synthese und Kristallstruktur von Ba4.5 Ca1.5 La2 Fe4 O15, Ba5 Ca Eu2
Fe4 O15 und Ba5 Ca Nd2 Co4 O15
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              84
_journal_page_last               88
_journal_paper_doi               10.1002/zaac.19926170113
_journal_volume                  617
_journal_year                    1992
_chemical_formula_structural     'Ba5 Ca Nd2 Co4 O15'
_chemical_formula_sum            'Ba5 Ca Co4 Nd2 O15'
_chemical_name_systematic
;
Pentabarium calcium dineodymium tetracobalt(III) oxide
;
_space_group_IT_number           186
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.6043(19)
_cell_length_b                   11.6043(19)
_cell_length_c                   6.8389(27)
_cell_volume                     797.5
_refine_ls_R_factor_all          0.085
_cod_database_code               2002596
Zur Kenntnis von Sr2 Bi3 V3 O14
Boje, J; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 618 (1992) 39–42; doi:10.1002/zaac.19926180108

data_2002597
_publ_section_title              'Zur Kenntnis von Sr2 Bi3 V3 O14'
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              39
_journal_page_last               42
_journal_paper_doi               10.1002/zaac.19926180108
_journal_volume                  618
_journal_year                    1992
_chemical_formula_structural     'Sr2 Bi3 V3 O14'
_chemical_formula_sum            'Bi3 O14 Sr2 V3'
_chemical_name_systematic        'Distrontium tribismuth trivanadium oxide'
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                97.462(33)
_cell_angle_beta                 98.704(25)
_cell_angle_gamma                110.989(20)
_cell_formula_units_Z            2
_cell_length_a                   7.0838(29)
_cell_length_b                   7.1732(32)
_cell_length_c                   14.1067(54)
_cell_volume                     648.3
_refine_ls_R_factor_all          0.077
_cod_database_code               2002597
Na2 Ba Cu V2 O8: ein neuer Strukturtyp der Alkali-Erdalkalimetall Kupfer-Oxovanadate
Postel, M von; Mueller-Buschbaum, Hk; Zeitschrift fuer Anorganische und Allgemeine Chemie 618 (1992) 107–110; doi:10.1002/zaac.19926180119

data_2002598
_publ_section_title
;
Na2 Ba Cu V2 O8: ein neuer Strukturtyp der Alkali-Erdalkalimetall
Kupfer-Oxovanadate
;
_journal_name_full
;
Zeitschrift fuer Anorganische und Allgemeine Chemie
;
_journal_page_first              107
_journal_page_last               110
_journal_paper_doi               10.1002/zaac.19926180119
_journal_volume                  618
_journal_year                    1992
_chemical_formula_structural     'Na2 Ba Cu (V O4)2'
_chemical_formula_sum            'Ba Cu Na2 O8 V2'
_chemical_name_systematic        'Disodium barium copper bis(vanadate)'
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.344(27)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.4329(32)
_cell_length_b                   5.6858(52)
_cell_length_c                   14.0488(32)
_cell_volume                     752.9
_refine_ls_R_factor_all          0.066
_cod_database_code               2002598
Zur Kristallstruktur von Ba3 Ln4 O9 (Ln=Dy, Er, Y/Yb)
Mueller-Buschbaum, Hk; Schrandt, O; Journal of Alloys Compd. 191 (1993) 151–154; doi:10.1016/0925-8388(93)90288-X

data_2002599
_publ_section_title
;
Zur Kristallstruktur von Ba3 Ln4 O9 (Ln=Dy, Er, Y/Yb)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              151
_journal_page_last               154
_journal_paper_doi               10.1016/0925-8388(93)90288-X
_journal_volume                  191
_journal_year                    1993
_chemical_formula_structural     'Ba3 Dy4 O9'
_chemical_formula_sum            'Ba3 Dy4 O9'
_chemical_name_systematic        'Tribarium tetradysprosium oxide'
_space_group_IT_number           146
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3'
_symmetry_space_group_name_H-M   'R 3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   6.129(1)
_cell_length_b                   6.129(1)
_cell_length_c                   25.282(6)
_cell_volume                     822.5
_refine_ls_R_factor_all          0.029
_cod_original_sg_symbol_H-M      'R 3 H'
_cod_database_code               2002599